Research Article  Open Access
Jinghui Li, Fuguo Li, Junzhe Dong, Zhanwei Yuan, Shuo Zhang, "Micromechanical Behavior of SingleCrystal Superalloy with Different Crystal Orientations by Microindentation", Journal of Nanomaterials, vol. 2015, Article ID 759753, 15 pages, 2015. https://doi.org/10.1155/2015/759753
Micromechanical Behavior of SingleCrystal Superalloy with Different Crystal Orientations by Microindentation
Abstract
In order to investigate the anisotropic micromechanical properties of singlecrystal nickelbased superalloy DD99 of four crystallographic orientations, (001), (215), (405), and (605), microindentation test (MIT) was conducted with different loads and loading velocities by a sharp Berkovich indenter. Some material parameters reflecting the micromechanical behavior of DD99, such as microhardness , Young’s modulus , yield stress , strain hardening component , and tensile strength , can be obtained from loaddisplacement relations. and of four different crystal planes evidently decrease with the increase of . The reduction of is due to dislocation hardening while is related to interplanar spacing and crystal variable. of (215) is the largest among four crystal planes, followed by (605), and (001) has the lowest value. of (215) is the lowest, followed by (605), and that of (001) is the largest. Subsequently, a simplified elasticplastic material model was employed for 3D microindentation simulation of DD99 with various crystal orientations. The simulation results agreed well with experimental, which confirmed the accuracy of the simplified material model.
1. Introduction
In recent years, singlecrystal nickelbased superalloys are widely used as blade of modern gas turbine aeroengines, as they significantly raise the operation temperature and efficiency due to excellent mechanical properties in service [1–6]. Their excellent hightemperature properties are superior to conventional cast alloys, such as hightemperature creep and oxidationresistant performance, which results from the elimination of grain boundaries in singlecrystal alloys. However, the absence of grain boundaries also leads to orientationdependent material response [7–9]. To date, a lot of researches concerned about different orientation of singlecrystal nickelbased superalloys have been done. Caron et al. [10] investigated the anisotropic creep behavior of some advanced superalloys (CMSX2, Alloy 454, MXON, and CMSX4) in the temperature ranging from 1033 to 1323 K. He et al. [11] discussed the creep/fatigue damage characteristics of DD6 and the results show the capability of DD6 to avoid fatigue damage in [011] direction is better than that in [001] direction. Yi et al. [12] gave modeling process of tertiary creep of singlecrystal superalloy along different orientations. Wu et al. [13] made extensile and compression tests at different temperatures on DD8 with various strain rates and the results indicate that the tendency to the plastic deformation inhomogeneity decreases in the order of [011], [001], and [111]. The previous investigations mainly concentrated on the fatigue life and creep properties with different orientations, while other fundamental performances of materials, such as hardness, Young’s modulus, and yield stress are rarely focused on.
Conventional tensile tests are difficult to conduct at nanoand microscales to determine orientation dependent behavior. Microindentation can be an alternative approach to tension or compression to probe the micromechanical properties, such as elastic modulus and hardness. Due to its precise measurement and advantages of celerity, accuracy, and nondestructiveness [15], it will become increasingly popular in the future. However, thorough understanding of materials behavior under indenter cannot be achieved just through MIT; for example, the equivalent stress and strain cannot be obtained directly by indentation.
FEM may be used as a supplement to solve complex 3D problems and more information can be extracted from microindentation simulation [16–18]. Lim and Munawar Chaudhri [19] investigated microindentation hardness of individual grains [(110) and (111) surfaces] of a polycrystalline copper using a spherical indenter and reported the indentation hardness in copper with different orientations to be very similar. Liu et al. [20] performed nanoindentation simulation using 3D elasticplastic crystal plasticity FEM on singlecrystal copper specimens on three orientations [(011), (100), and (111)] using a conical indenter and reported twofold, fourfold, and sixfold symmetries on (011), (100), and (111) faces, respectively. Fivel et al. [21] developed a 3D model to combine discrete dislocations with FEM for nanoindentation simulation on singlecrystal copper. However, most of these researches were based on material properties of singlecrystal data obtained from tensile testing at macroscale. In fact, it is essential to extract these parameters at micrometer scale.
In this paper, MIT were conducted on crystal planes of nickelbased singlecrystal DD99 to investigate its micromechanical properties. Subsequently, a FEM model based on the results of MIT was implemented in 3D ABAQUS/Explicit to prove the accuracy of this FEM model.
2. Calculation Methods
2.1. ElasticPlastic Properties
The loaddisplacement response obtained by microindentation contains information about the elastic and plastic deformation of the indented materials. Therefore, it is often regarded as “fingerprint” of materials’ properties under identification [22]. Mechanical properties, such as the hardness and Young’s modulus, can be readily extracted from the loaddisplacement curves. In general, plastic behavior of metals can be characterized by a powerlaw description, as shown in Figure 1. A simplified elasticplastic, true stressstrain behavior can be expressed as
When is equal to , can be deduced as follows:
Thus, 1 can be rewritten as follows:
In order to describe the mechanical properties of a powerlaw material, Young’s modulus , yield stress , and strain hardening exponent are needed.
The typical  curve of microindentation test is shown in Figure 2. Two important parameters (maximum indentation depth and maximum load ) can be obtained from the curve. According to Kick’s law, the loading curve of indentation can be expressed as
According to the model proposed by Oliver and Pharr [23, 24], unloading curve can be interpreted as
The relationship between the apparent modulus and Young’s modulus is as follows: and are Young’s modulus and Poisson’s ratio of the indenter whose values are 1141 GPa and 0.07 for diamond indenter, respectively [25].
According to King [26], has the form and can be obtained by the following equations, respectively: where is a constant related with indenter, whose value is 24.56 for Berkovich indenter, and is a coefficient with value of 0.75 for Berkovich indenter [27, 28].
The next task is to find the yield stress and strain hardening exponent . The method used to obtain and is dimensional analysis proposed by Y. T. Cheng and C. M. Cheng and Tunvisut et al. [29–33]. For a sharp indenter (Berkovich indenter in this paper), the load can be related with the following parameters [34]:
According to theorem in dimensional analysis, the equation above can be rewritten as function is independent of when strain is equal to 0.033 [34]. And can be obtained as
Similarly, the unloading slope can be described as follows at :
Finally, after plugging value of and into 3, can be calculated. Thus, one can obtain the elasticplastic model characterized by a powerlaw function based on 1 and 2.
2.2. Tensile Strength
The ultimate tensile strength characterizes the resistance of largest uniform plastic deformation. The tensile strength is usually determined by uniaxial tensile test: the highest point of the stressstrain curve is the tensile strength. However, it can also be calculated by MIT.
In the stage of uniform plastic deformation stage, load is as follows:
The result of differential calculation of 15 is
When nonuniform deformation such as necking occurs on certain part of materials, reaches its maximum value and . According to 16, it can be induced that
It has the following relationship, according to 18:
According to 19, can be calculated and it is equal to , which has been confirmed by [35]. Consider
Its formula is
According to 21 and 22, can be calculated:
2.3. Microhardness
Hardness is an ability of resistance to permanent (plastic) deformation. It represents the overall mechanical properties of materials. For example, hardness is related to other mechanics parameters, such as Young’s modulus, yield stress, and strain hardening component [36]. Besides, many references have shown that the intrinsic material length scale characterizing size scale can be identified from microhardness [37–41]. It has been found that the microhardness of materials is significantly higher that the microhardness and, furthermore, the correlation of microhardness and the indentation depth implies that the materials strength depends on both the absolute specimen size and strain gradients. Therefore, the results of the microhardness provide a new implication for the strain gradientdependent constitutive equations in continuum plasticity theory. This has led to the development of phenomenological or mechanismbased strain gradient plasticity (SGP) theories, which have been used to interpret the size dependence of hardness from the micro to nanoscales.
Shim et al. [42] guessed the yield strength very roughly based on the hardness values from Berkovich indentations. Nix and Gao [43] showed that equivalent stress () has the following relationship with hardness: . As a testing method under micro and nanoscale, MIT plays an important role in the evaluation of microhardness and the microhardness can be obtained as follows:
3. Experimental and Simulation Procedures
3.1. Experimental Procedure
The nominal chemical compositions of asreceived singlecrystal nickelbased superalloy DD99 (5 mm × 5 mm × 3 mm rectangle block) which has its crystal plane (001) marked in advance are shown in Table 1.

Although nickelbased single crystal has the optimum performance along crystal orientation [001] [14], there inevitably exist misorientations for actual engineering application. Moreover, as the structures of production, such as blade parts of aeroengine, are complicated, it is difficult to guarantee each plane of the product is parallel to [001]. In order to investigate the orientation dependent properties and provide performance reference of different planes for engineering applications in the future, the specimens of DD99 were subjected to wireelectrode cutting with angle of 30°, 45°, and 60° to crystal plane (001), as shown in Figures 3(a), 3(b), and 3(c). The red lines in Figure 3 represent molybdenum wire used in wireelectrode cutting and the cutting curve is parallel to [010].
(a)
(b)
(c)
The cutting specimens along with the original one with crystal plane (001) were carefully ground with sand paper. Then, they were polished with 1.5 μm diamond to mirror finish. Subsequently, the specimens were etched with corrosives (5 g CuSO_{4} + 20 mL HCl + 100 mL H_{2}O) for 15 s to reduce the influence of surface hardening. Finally, MIT was performed using the commercial MCT W501 equipped with a Berkovich diamond indenter at room temperature. The test condition was shown in Table 2. There are four different loading velocities and under each of them nine different maximum loads were conducted. Notably, each test was conducted five times and the average values were calculated in order to eliminate the errors.

3.2. Simulation Procedure
In the researches of Li et al. [44] and Yuan et al. [45], the axisymmetric 2D was created by using the quadrilateral elements to simulate the indentation process and the  line of FEM is slightly higher than that of experiments. Walter and Mitterer [46] found that 2D model predicts higher scatter and relatively higher mean Young’s modulus compared to 3D model. According to researches from FEM simulation of indentation, it can be concluded that the main differences between 2D and 3D model are in the following two aspects.
In terms of the shape of indenter, the Berkovich indenter of 2D model is represented by a straight with an angle of 70.3° to axis of symmetry, indicating the indenter itself as a whole is conical. In contrast, the real shape of Berkovich indenter is triangular pyramid. Considering the boundary conditions, circumferential displacement in 2D model is constrained and only the displacement in radial direction is permitted. By comparison, constrained circumferential displacement just appears on the symmetry plane and deformation can be expanded in both circumferential and radial direction within matrix in 3D model. Considering above variations and the fact that 2D model cannot be utilized to discuss the orientation dependent properties due to its rotational symmetry, a 3D simulation seems preferable, even though computational time is considerably higher.
The Berkovich indenter is a triangularbased pyramid having a threefold symmetry. The load is applied along the axis of the indenter; thus the load symmetry is the same as the geometric one. For these considerations, a threedimensional model is defined only by onethird of the entire system. The 3D model setup is shown in Figure 4. In the simulations, the indenter is modeled as a rigid body. This is justified as the diamond indenter has a modulus of 1141 GPa. In this paper, the dimension of material in FEM model is 2 mm × 2 mm × 1 mm, which is much larger than maximum indentation displacement. As for the mesh section, size of mesh is generally a compromise between the computational cost and the solution accuracy. Based on various deformation levels, a finer mesh is used near the indenter tip and a coarser mesh for farther regions. And the element of material is C3D8R, while that of indenter is R3D3. The effect of friction coefficient on the nanoindentation behavior has been investigated by Liu et al. [47], illustrating that the friction does not change the loaddisplacement relationship. A lower friction contact pair is defined by two contact surfaces with associated nodes between the indenter and the material. In addition, boundary conditions are defined as an element on two symmetry planes parallel to indenter movement direction constrained, only able to expand along radical and axial direction with the help of cylindrical coordinate. But the elements on the bottom of material were defined as having no displacement in any direction.
4. Experimental Results and Analysis
4.1. Microhardness and Tensile Strength
The loaddisplacement curves ( curves) of crystal plane (405) under loading velocity of 17.284 mN/s are shown in Figure 5. It can be found that curves of various loads show similar shape, which indicates a better repeatability of indentation tests. Different from the nanoindentation test, no “popin” size by the abrupt plastic flow generated by the high density of dislocation nucleation and propagation is observed in microindentation [48]. Based on these curves, micromechanical parameters (, , , , and ) can be obtained according to equations mentioned in Section 2.
Based on 24, microhardness of four different crystal planes ((001), (215), (405), and (605)) has been calculated. The results are shown in Figure 6.
(a)
(b)
(c)
(d)
It can be seen from Figure 6 that of each crystal plane under different velocities is almost the same although data of (001) with 51.8527 mN/s derives from others slightly, which indicates that microindentation loading velocities had little influence on the results of . And the similar phenomenon was founded in Ti6Al4V alloy [49]. Therefore, loading velocity of 17.2842 mN/s was used in the following investigation. of different crystal planes corresponding to 17.2842 mN/s was shown in Figure 7.
According to Figure 7, of four crystal planes evidently decreases with the increase of maximum load. The phenomenon that indentation depth increases with increase of maximum load confirms the reduction of . In addition, the apparent drop of occurs when the loads are less than 2000 mN. When loads are above 2000 mN, their values reduce up to 8%. This phenomenon is attributed to indentation size effects (ISE) caused by geometrically necessary dislocations (GNDs). At the micro/nanoscales, GNDs are large enough and arranged periodically and regularly to cause strong obstacles to slip. GNDs have a strengthening effect on hardness and enhance indurations of material [50]. But values of GNDs have a decreasing tendency with the increase of , which can be demonstrated by the equation of density of GNDs () for a Berkovich indenter: where is the angle between surface of the indenter and plane of the surface with the value of 19.7° for Berkovich indenter [27].
Moreover, Nix and Gao proposed a new model of and , based on Taylor dislocation and geometrically necessary dislocation model [43, 51]: where is a length that characterizes the depth dependence of hardness: where is a constant, whose value is 0.3–0.5.
According to 26 and 27, one can find that when is low, is of small value correspondingly. Thus of region under indenter is considerable and the measured values of are large. When load is relatively higher, is in a lower amount and its hardening effect is relatively small on , when remains almost stable.
As for each crystal plane, of (001) is close to that of (405), while it is higher than those of (215) and (605). (405) has the largest values of , followed by (001) and (215), which can be explained by dislocation hardening mechanism. It is well known that there are four mechanisms existing in metallic: solid solution hardening, dislocation hardening, boundary hardening, and precipitation hardening. In this paper, single crystal that has no crystal boundary was investigated and the solid solution and precipitation hardening can be ascribed to dislocation movement. Therefore, dislocation hardening is the dominant factor on . In the literature, the density equation of dislocation () has been proposed:
The statistically stored dislocations density on four crystal planes can be calculated through 29, as shown in Figure 8. It can be seen that (001) has the largest dislocation density among these crystal planes, and second for (405), the lowest for (215). Compared with of four crystal planes in Figure 7, it is reasonable that of (605) and (215) is lower than those of other two planes. Because dislocation density is lower, hardening effect caused by dislocation is weaker. However, with regard to of (001) and (405), of (405) is larger than that of (001), although of (001) is higher. This phenomenon can be explained by the following facts. For metallic materials with FCC crystal structure, slip easily takes place on the closepacked octahedral planes and in the closepacked directions. Generally, for FCC lattice there are four slip planes and three corresponding slip directions, namely, posing twelve slip systems. But there are eight equivalent slip systems on (001) planes, while there is only one equivalent slip system on (405), (605), and (215). Compared with (405), dislocation may extend through different slip systems and hardly pile up due to more slip systems on (001). Therefore, of (001) is a little lower than that of (405).
4.2. Young’s Modulus
Of the various unique mechanical properties of materials, Young’s modulus, which is a measure of elasticity, has attracted particular attention. Figure 9 shows Young’s modulus of four different crystal planes ((001), (215), (405), and (605)) calculated according to 6.
(a)
(b)
(c)
(d)
It can be seen from Figure 9 that the calculated of each crystal plane under different velocities has similar values, illustrating that microindentation loading speeds had little influence on the results of . And the similar phenomenon was also found in Ti6Al4V alloy [49]. Therefore, loading speed with value of 17.2842 mN/s was used for the following investigation.
Figure 10 gives the values of from different crystal planes under the loading speed of 17.2842 mN/s. As shown in Figure 10, it can be concluded that decreases with the increase of on the whole.
Compared with of the same planes, also decreases rapidly with loads below 2000 mN. And its values remain almost the same when subjected to the higher loads. The induced damage is responsible for this phenomenon. The reduction of Young’s modulus is typically regarded as a characterization of damage evolution and accumulation. When dislocations accumulate or pile up in a certain region, it is easy for stress to concentrate and eventually surpass its threshold. Thus, damage can be easily generated and extended under indentation load, resulting in elastic properties weakening and decreasing. In addition, when loads are below 2000 mN, each of curves falls quickly due to the high values of (Figure 8) and the corresponding rapid damage accumulation. However, when the loads are around 4000 mN, fluctuation of is steady and has no obvious effect on variation of .
For each crystal plane, of (001) is larger than others and (215) has the lowest value. Crystalline structure and theory of metallic plasticity contribute qualitatively to the explanation of diverse from different crystal plane. For example, for cubic system, the expression for the interplanar spacing () is as follows: where is 0.358 nm for DD99.
According to 30, the interplanar spacing of (001), (215), (405), and (605) is 0.358 nm, 0.0703 nm, 0.06 nm, and 0.0493 nm, respectively. The greater the interplanar spacing is, the larger the density of atoms on this crystal plane is. The greater interplanar spacing is significantly efficient in driving the movement of atoms on the crystal plane, which poses a larger . However, this explanation does not work for (405) in comparison with that of (215); this phenomenon needs further research.
According to theory of metallic plasticity, the crystal can be also obtained through stiffness coefficient and crystal indices [52]. For cubic system, can be calculated as the following equation:
For the same material, with different crystal orientation and planes mainly depends on
For crystal nickelbased DD99, value of is negative. According to 32, the value of (001) is 0, which is the smallest one among four crystal planes, while (605) is having the largest data of 0.24187. So (001) has the largest , but of (605) is relatively lower.
4.3. ElasticPlastic Constitutive Model
According to equations in Section 2.1, the values of and of (405) under different loads are shown in Figure 11. It is evident that they remain constant regardless of the different loads.
As shown in Figure 12, values of and are shown in bar graph. It can be found that of (215) is the largest, followed successively by (605) and (001). However, the values of show the opposite tendency. That is, of (215) is the lowest, followed by (605), and that of (001) is the largest.
It is well known that is the strength assessing the ability to resist the plastic deformation. And for materials with power hardening law, is used as a parameter evaluating a kind of ability that maintains homogeneous deformation. The higher of certain material, the better compatibility of deformation of material. The differences of on four crystal planes can be explained by Schmid’s law.
In Figure 13, a typical uniaxial tensile stress exerted on a metal cylinder is shown. is the area normal to the axial force and is the area of the slip plane on which the resolved shear force is acting. is the angle between and the normal to the slip plane area , and is the angle between and the slip direction. For activating dislocations to move in the slip system, a sufficient resolved shear stress () in the slip direction must be produced, and is computed as
This is called Schmid’s law. is called Schmid factor and defined as follows: , , and are shown in Table 3.

is a constant for a previous known lattice, and independent of the orientation of , it can be inferred that is larger, if is smaller according to 33 and 34. Therefore, the fact that of (215) is larger than that of (605), which is followed by (405), can be understandable, because of (215), (605), and (405) increases sequentially. With particular emphasis on of (001) which is the lowest, it has eight equivalent slip systems, while there is only one equivalent slip system on (405), (605), and (215). For FCC singlecrystal structure, Schmid’s law is no longer valid, regardless of potential slip systems. When value and orientation of are appropriate, of two or more slip systems can be achieved, which makes the situation complicated, and Schmid law does not work anymore.
For (001) crystal having eight equivalent slip systems and a relatively lower , the dislocations can extend easily and the deformation resistance is low, resulting in better compatibility of uniform deformation. So, it has the largest . With regard to (215), (605) and (405) who yield only one equivalent slip system, the yield strength decrease in order, namely, compatibility of deformation of (405) is the best, followed by (605). And that of (215) is the worst of all. Therefore, of (405) is larger than that of (605).
Based on 2 and 23, and along with other parameters representing elasticplastic properties can be obtained in Table 4.

Mechanical property parameters, , , , and , were obtained from microindentation experimental data; thus the elasticplastic equations of DD99 on different crystal planes can be obtained as
5. Verification of ElasticPlastic Model
Simulation calculations have been performed by using the commercial finite element software ABAQUS. The experimental and FEM results of 500 mN, 2500 mN, and 4500 mN on crystal plane (405) were shown in Figure 14. The experimental curves agreed well with computed  curves, which indicates that above elasticplastic equations of DD99 obtained by MIT are valid and 3D FEM model of indentation can fully describe and simulate microindentation process.
Although FEM results deviate from experimental results slightly, it is of great importance to focus on their difference. In order to illustrate cause of deviation to achieve better simulations in the future, experimental and FEM results of 2500 mN on different crystal planes were shown in Figure 15.
(a)
(b)
(c)
(d)
As shown in Figure 15, it can be concluded that FEM results seem like experimental data moving right. To be more specific, FEM results have various degrees of deviation from experimental results during the loading process, especially in the middle process of the loading. This phenomenon can be explained by Kick’s law (Equation 4) and decrease of along with increase of .
There is a relationship between and originally suggested by Tabor [53]:
According to 9 and 24, can be expressed as follows: where is a constant.
Therefore, Kick’s law seems to be reasonable. However, microindentation test is not an ideal plastic deformation process. ISE exists in the process of microindentation as discussed above, resulting in decrease of . As is the function of shown in 26, is also a function of according to 37. And the relationship between and is no longer quadratic function. When the load is low, ISE is obvious [54] and error of results from Kick’s law is larger compared with those under high load. In order to prove it, the experimental and FEM results of (405) under 500 mN and 2500 mN were utilized, as shown in Figure 16. Besides, the lower load yields a poor accuracy between simulated and experimental results in comparison with the higher load, which may be due to the transition of contact modes from purely elastic under lower loads to elastic/plastic under higher loads. Jian et al. [22, 55, 56] have maintained that the behaviors during indentation can be roughly divided into two stages by the variation of microhardness. Namely, the hardness initially increases with the penetration depth due to the transition between purely elastic and elastic/plastic contact.
(a)
(b)
Also the decrease of along with increase of may also be blamed for the difference between experimental and FEM results. In FEM model, the selection of is a complicated question. As shown in Figure 10, of four crystal planes decreases with the increase of due to damage, actually changes a little with high load, and the value of with high load is used in FEM model. In the preliminary stage of indentation, of materials is higher than that used in FEM model. According to stressstrain relationship in the elastic stage, the higher is corresponding to the smaller . So of FEM is larger than that of experimental data.
With regard to unloading process, the slope of unloading curve is related with according to 13. And it can be found that all the unloading curves of FEM results are parallel to that of experimental data (Figure 15), indicating that the difference of unloading process is attributed to the error of in loading process and the selection of in FEM model is reasonable.
In order to interpret the matching degree of  curves in FEM results and experimental data quantitatively, the predictability of the applied load is further quantified employing standard statistical parameters correlation coefficient (). was a commonly used statistic and provides information on the dispersion between the experimental and the computed values. It was expressed as [57, 58] where is the experimental indenter load, is the predicted indenter load, and and are the mean values of and , respectively.
According to literature [59], the predictability of the matching degree of  curves can also be quantified by the average absolute relative error (AARE) and the results of and AARE are as shown in Table 5:

6. Conclusions
Microindentation measurements using a sharp Berkovich indenter on singlecrystal nickelbased superalloy DD99 of four crystallographic orientations, that is, (001), (215), (405), and (605), were made to determine the loaddisplacement relations. Some material parameters reflecting the micromechanical behavior of DD99, such as microhardness , Young’s modulus , yield stress , strain hardening component , and tensile strength , can be obtained from loaddisplacement relations. Subsequently, the process of MIT is simulated using 3D FEM based on the above parameters. Eventually, the influence of crystal orientations on micromechanical properties can be concluded as follows.(1) of four different crystal planes evidently decreases with the increase of . The crystal plane (405) has the largest microhardness values, followed by (001). of (215) is the lowest. This phenomenon is related to dislocation hardening.(2) of these planes decreases with the increase of . (001) has the largest , followed by (405). And of (215) is the lowest, which is attributed to the fact that (001) has the largest interplanar spacing and smallest crystal variable.(3) is inversely correlated with on all these planes. of (215) is the largest among four crystal planes, followed by (605), and (001) has the lowest value. However, of (215) is the lowest, followed by (605), and that of (001) is the largest. It can be explained by Schmid’s factor () and the larger crystal plane has and the lower it possesses. In addition, on four planes was calculated and it is similar except for (215).
Although FEM results deviate slightly from experimental results, they can be used as sufficient evidences indicating the accuracy of 3D FEM model and material elasticplastic model founded from MIT.
Nomenclature
:  Crosssectional area, mm^{2} 
:  Crosssectional area corresponding to , mm^{2} 
:  Lattice constant 
and :  Fitting coefficients 
:  Burgers vector 
:  A variable related to material properties as well as indenter geometry 
:  Constraint factor 
:  Elastic modulus, MPa 
:  Effective elastic modulus of damaged material, MPa 
:  Microhardness, kgmm^{−2} 
:  microhardness regardless of strain gradient plasticity, kgmm^{−2} 
:  Indenter displacement, μm 
:  Residual depth after unloading, μm 
, , and :  Miller indices 
:  Schmid factor 
:  Strain hardening exponent 
:  Indenter load, mN 
:  Strength coefficient 
, , and :  Independent elastic compliance constant. 
:  True strain 
:  Corresponding strain to initial yield stress 
:  Strain corresponding to 
:  Initial yield stress, MPa 
:  Representative stress, MPa 
:  Ultimate tensile strength, MPa 
:  Flow stress, MPa 
:  Poisson’s ratio 
:  Shear modulus, MPa 
:  Density of statistically stored dislocations. 
Conflict of Interests
The authors declare that there is no conflict of interests regarding the publication of this paper.
Acknowledgments
The authors would like to express their sincere thanks for the research grants supported by the National Natural Science Foundation of China (Grant no. 51275414), the Aeronautical Science Foundation of China (Grant no. 2011ZE53059), and the Graduate Starting Seed Fund of Northwestern Polytechnic University (Grant no. Z2014007).
References
 G. L. Erickson, “Single crystal nickelbased superalloy,” Google Patents, 1994. View at: Google Scholar
 A. Sato, Y.L. Chiu, and R. C. Reed, “Oxidation of nickelbased singlecrystal superalloys for industrial gas turbine applications,” Acta Materialia, vol. 59, no. 1, pp. 225–240, 2011. View at: Publisher Site  Google Scholar
 C. Lane, “Introduction,” in The Development of a 2D Ultrasonic Array Inspection for Single Crystal Turbine Blades, Springer Theses, pp. 1–12, Springer, 2014. View at: Publisher Site  Google Scholar
 J.J. Yu, X.F. Sun, N.R. Zhao, T. Jin, H.R. Guan, and Z.Q. Hu, “Effect of carbon on microstructure and mechanical properties of DD99 single crystal superalloy,” Transactions of Nonferrous Metals Society of China, vol. 16, pp. 1973–1977, 2006. View at: Google Scholar
 Z.H. Yu, L. Liu, X.B. Zhao, W.G. Zhang, J. Zhang, and H.Z. Fu, “Advance in research of carbon effect on single crystal Nibase superalloy,” Foundry, vol. 58, no. 9, p. 10, 2009. View at: Google Scholar
 T.B. Wu, X.F. Yu, Y.L. Man et al., “Burning loss of carbon and influence factors of oxygen content during vacuum induction melting,” Foundry, vol. 62, no. 1, pp. 1–3, 2013. View at: Google Scholar
 J. S. Wan and Z. F. Yue, “A lowcycle fatigue life model of nickelbased single crystal superalloys under multiaxial stress state,” Materials Science and Engineering A, vol. 392, no. 12, pp. 145–149, 2005. View at: Publisher Site  Google Scholar
 H. U. Hong, J. G. Yoon, B. G. Choi, I. S. Kim, and C. Y. Jo, “On the mechanism of secondary reaction zone formation in a coated nickelbased singlecrystal superalloy containing ruthenium,” Scripta Materialia, vol. 69, no. 1, pp. 33–36, 2013. View at: Publisher Site  Google Scholar
 D. Shi, C. Dong, and X. Yang, “Constitutive modeling and failure mechanisms of anisotropic tensile and creep behaviors of nickelbase directionally solidified superalloy,” Materials & Design, vol. 45, pp. 663–673, 2013. View at: Publisher Site  Google Scholar
 P. Caron, T. Khan, Y. Ohta, and Y. Nakagawa, “Creep deformation anisotropy in single crystal superalloys,” in Superalloys 1988, pp. 215–224, TMS, Warrendale, Pa, USA, 1988. View at: Google Scholar
 M. He, H. Li, and J. Nie, “An investigation on creep/fatigue damage characteristics of singlecrystal DD6 at high temperature,” Gas Turbine Experiment and Research, vol. 15, no. 2, pp. 24–27, 2002. View at: Google Scholar
 J. Z. Yi, C. J. Torbet, Q. Feng, T. M. Pollock, and J. W. Jones, “Ultrasonic fatigue of a single crystal Nibase superalloy at 1000 °C,” Materials Science and Engineering A, vol. 443, no. 12, pp. 142–149, 2007. View at: Publisher Site  Google Scholar
 X. Wu, J. H. Zhang, J. L. Liu, T. Jin, Y. B. Xu, and Z. Q. Hu, “Plastic deformation inhomogeneity in a single crystal nickelbase superalloy,” Materials Science and Engineering A, vol. 325, no. 12, pp. 478–483, 2002. View at: Publisher Site  Google Scholar
 S. L. Semiatin and T. R. Bieler, “The effect of alpha platelet thickness on plastic flow during hot working of Ti6Al4V with a transformed microstructure,” Acta Materialia, vol. 49, no. 17, pp. 3565–3573, 2001. View at: Publisher Site  Google Scholar
 M. Jamal and M. Morgan, “Determination of the mechanical properties of thermally treated recycled glass based on nanoindentation measurement and FEM supported simulation,” Key Engineering Materials, vol. 581, pp. 472–477, 2014. View at: Publisher Site  Google Scholar
 W. B. Lee and Y. P. Chen, “Simulation of microindentation hardness of FCC single crystals by mechanismbased strain gradient crystal plasticity,” International Journal of Plasticity, vol. 26, no. 10, pp. 1527–1540, 2010. View at: Publisher Site  Google Scholar
 L. Wang, X. H. Zhong, J. S. Yang et al., “Finite element simulation of surface microindentation behavior of yttria stabilized zirconia thermal barrier coatings with microstructural characteristic of columnar grains and subgrains based on a nonlinear contact model,” Computational Materials Science, vol. 82, pp. 244–256, 2014. View at: Publisher Site  Google Scholar
 W. Z. Yao, C. E. Krill III, B. Albinski, H.C. Schneider, and J. H. You, “Plastic material parameters and plastic anisotropy of tungsten single crystal: a spherical microindentation study,” Journal of Materials Science, vol. 49, no. 10, pp. 3705–3715, 2014. View at: Publisher Site  Google Scholar
 Y. Y. Lim and M. Munawar Chaudhri, “The influence of grain size on the indentation hardness of highpurity copper and aluminium,” Philosophical Magazine A, vol. 82, no. 10, pp. 2071–2080, 2002. View at: Publisher Site  Google Scholar
 Y. Liu, S. Varghese, J. Ma, M. Yoshino, H. Lu, and R. Komanduri, “Orientation effects in nanoindentation of single crystal copper,” International Journal of Plasticity, vol. 24, no. 11, pp. 1990–2015, 2008. View at: Publisher Site  Google Scholar
 M. C. Fivel, C. F. Robertson, G. R. Canova, and L. Boulanger, “Threedimensional modeling of indentinduced plastic zone at a mesoscale,” Acta Materialia, vol. 46, no. 17, pp. 6183–6194, 1998. View at: Publisher Site  Google Scholar
 S.R. Jian, J.Y. Juang, C.W. Luo, S.A. Ku, and K.H. Wu, “Nanomechanical properties of GaSe thin films deposited on Si(1 1 1) substrates by pulsed laser deposition,” Journal of Alloys and Compounds, vol. 542, pp. 124–127, 2012. View at: Publisher Site  Google Scholar
 W. C. Oliver and G. M. Pharr, “Improved technique for determining hardness and elastic modulus using load and displacement sensing indentation experiments,” Journal of Materials Research, vol. 7, no. 6, pp. 1564–1580, 1992. View at: Publisher Site  Google Scholar
 G. M. Pharr, W. C. Oliver, and F. R. Brotzen, “On the generality of the relationship among contact stiffness, contact area, and elastic modulus during indentation,” Journal of Materials Research, vol. 7, no. 3, pp. 613–617, 1992. View at: Google Scholar
 N. Janakiraman and F. Aldinger, “Indentation analysis of elastic and plastic deformation of precursorderived SiCN ceramics,” Journal of the European Ceramic Society, vol. 30, no. 3, pp. 775–785, 2010. View at: Publisher Site  Google Scholar
 R. B. King, “Elastic analysis of some punch problems for a layered medium,” International Journal of Solids and Structures, vol. 23, no. 12, pp. 1657–1664, 1987. View at: Publisher Site  Google Scholar
 M. He, F. Li, J. Cai, and B. Chen, “An indentation technique for estimating the energy density as fracture toughness with Berkovich indenter for ductile bulk materials,” Theoretical and Applied Fracture Mechanics, vol. 56, no. 2, pp. 104–111, 2011. View at: Publisher Site  Google Scholar
 J. Li, F. Li, M. He, F. Xue, M. Zhang, and C. Wang, “Indentation technique for estimating the fracture toughness of 7050 aluminum alloy with the Berkovich indenter,” Materials and Design, vol. 40, pp. 176–184, 2012. View at: Publisher Site  Google Scholar
 Y.T. Cheng and C.M. Cheng, “Relationships between hardness, elastic modulus, and the work of indentation,” Applied Physics Letters, vol. 73, no. 5, pp. 614–616, 1998. View at: Publisher Site  Google Scholar
 Y.T. Cheng and C.M. Cheng, “Scaling approach to conical indentation in elasticplastic solids with work hardening,” Journal of Applied Physics, vol. 84, no. 3, pp. 1284–1291, 1998. View at: Publisher Site  Google Scholar
 Y.T. Cheng and C.M. Cheng, “Can stressstrain relationships be obtained from indentation curves using conical and pyramidal indenters?” Journal of Materials Research, vol. 14, no. 9, pp. 3493–3496, 1999. View at: Publisher Site  Google Scholar
 Y.T. Cheng and C.M. Cheng, “Relationships between initial unloading slope, contact depth, and mechanical properties for conical indentation in linear viscoelastic solids,” Journal of Materials Research, vol. 20, no. 4, pp. 1046–1053, 2005. View at: Publisher Site  Google Scholar
 K. Tunvisut, N. P. O'Dowd, and E. P. Busso, “Use of scaling functions to determine mechanical properties of thin coatings from microindentation tests,” International Journal of Solids and Structures, vol. 38, no. 2, pp. 335–351, 2001. View at: Publisher Site  Google Scholar
 M. Dao, N. Chollacoop, K. J. van Vliet, T. A. Venkatesh, and S. Suresh, “Computational modeling of the forward and reverse problems in instrumented sharp indentation,” Acta Materialia, vol. 49, no. 19, pp. 3899–3918, 2001. View at: Publisher Site  Google Scholar
 J.Y. Kim, K.W. Lee, J.S. Lee, and D. Kwon, “Determination of tensile properties by instrumented indentation technique: representative stress and strain approach,” Surface and Coatings Technology, vol. 201, no. 7, pp. 4278–4283, 2006. View at: Publisher Site  Google Scholar
 X.L. Gao, “New expanding cavity model for indentation hardness including strainhardening and indentation size effects,” Journal of Materials Research, vol. 21, no. 5, pp. 1317–1326, 2006. View at: Publisher Site  Google Scholar
 H. Yuan and J. Chen, “Identification of the intrinsic material length in gradient plasticity theory from microindentation tests,” International Journal of Solids and Structures, vol. 38, no. 4647, pp. 8171–8187, 2001. View at: Publisher Site  Google Scholar
 H. Yuan and J. Chen, “The role of intrinsic material length scales in microindentation simulations,” Computational Materials Science, vol. 25, no. 12, pp. 253–263, 2002. View at: Publisher Site  Google Scholar
 R. K. A. AlRub and G. Z. Voyiadjis, “Analytical and experimental determination of the material intrinsic length scale of strain gradient plasticity theory from micro and nanoindentation experiments,” International Journal of Plasticity, vol. 20, no. 6, pp. 1139–1182, 2004. View at: Publisher Site  Google Scholar
 R. K. Abu AlRub and G. Voyiadjis, “Determination of the material intrinsic length scale of gradient plasticity theory,” International Journal for Multiscale Computational Engineering, vol. 2, no. 3, 24 pages, 2004. View at: Google Scholar
 G. Z. Voyiadjis and R. A. AlRub, “Determination of the material intrinsic length scale of gradient plasticity theory,” in IUTAM Symposium on Multiscale Modeling and Characterization of ElasticInelastic Behavior of Engineering Materials, vol. 114 of Solid Mechanics and Its Applications, pp. 167–174, Springer, Dordrecht, The Netherlands, 2004. View at: Publisher Site  Google Scholar
 S. Shim, J.I. Jang, and G. M. Pharr, “Extraction of flow properties of singlecrystal silicon carbide by nanoindentation and finiteelement simulation,” Acta Materialia, vol. 56, no. 15, pp. 3824–3832, 2008. View at: Publisher Site  Google Scholar
 W. D. Nix and H. Gao, “Indentation size effects in crystalline materials: a law for strain gradient plasticity,” Journal of the Mechanics and Physics of Solids, vol. 46, no. 3, pp. 411–425, 1998. View at: Publisher Site  Google Scholar
 J. Li, F. Li, M. He, F. Xue, M. Zhang, and C. Wang, “Indentation technique for estimating the fracture toughness of 7050 aluminum alloy with the Berkovich indenter,” Materials & Design, vol. 40, pp. 176–184, 2012. View at: Publisher Site  Google Scholar
 Z. Yuan, F. Li, P. Zhang, B. Chen, and F. Xue, “Mechanical properties study of particles reinforced aluminum matrix composites by microindentation experiments,” Chinese Journal of Aeronautics, vol. 27, no. 2, pp. 397–406, 2014. View at: Publisher Site  Google Scholar
 C. Walter and C. Mitterer, “3D versus 2D finite element simulation of the effect of surface roughness on nanoindentation of hard coatings,” Surface and Coatings Technology, vol. 203, no. 2021, pp. 3286–3290, 2009. View at: Publisher Site  Google Scholar
 Y. Liu, B. Wang, M. Yoshino, S. Roy, H. Lu, and R. Komanduri, “Combined numerical simulation and nanoindentation for determining mechanical properties of single crystal copper at mesoscale,” Journal of the Mechanics and Physics of Solids, vol. 53, no. 12, pp. 2718–2741, 2005. View at: Publisher Site  Google Scholar
 S.R. Jian, C.H. Tasi, S.Y. Huang, and C.W. Luo, “Nanoindentation popin effects of Bi_{2}Te_{3} thermoelectric thin films,” Journal of Alloys and Compounds, vol. 622, pp. 601–605, 2015. View at: Publisher Site  Google Scholar
 J. Cai, F. Li, T. Liu, and B. Chen, “Investigation of mechanical behavior of quenched Ti6Al4V alloy by microindentation,” Materials Characterization, vol. 62, no. 3, pp. 287–293, 2011. View at: Publisher Site  Google Scholar
 M. S. Park and Y. S. Suh, “Hardness estimation for pileup materials by strain gradient plasticity incorporating the geometrically necessary dislocation density,” Journal of Mechanical Science and Technology, vol. 27, no. 2, pp. 525–531, 2013. View at: Publisher Site  Google Scholar
 K. Durst, B. Backes, and M. Göken, “Indentation size effect in metallic materials: correcting for the size of the plastic zone,” Scripta Materialia, vol. 52, no. 11, pp. 1093–1097, 2005. View at: Publisher Site  Google Scholar
 H. Ledbetter and A. Migliori, “A general elasticanisotropy measure,” Journal of Applied Physics, vol. 100, no. 6, Article ID 063516, 2006. View at: Publisher Site  Google Scholar
 D. Tabor, The Hardness of Metals, Clarendon Press, Oxford, UK, 1951.
 J. Dong, F. Li, and C. Wang, “Micromechanical behavior study of α phase with different morphologies of Ti6Al4V alloy by microindentation,” Materials Science and Engineering: A, vol. 580, pp. 105–113, 2013. View at: Publisher Site  Google Scholar
 S.R. Jian and Y.Y. Lin, “Berkovich nanoindentationinduced dislocation energetics and popin effects in ZnSe thin films,” Journal of Alloys and Compounds, vol. 590, pp. 153–156, 2014. View at: Publisher Site  Google Scholar
 C.H. Tasi, Y.C. Tseng, S.R. Jian et al., “Nanomechanical properties of Bi_{2}Te_{3} thin films by nanoindentation,” Journal of Alloys and Compounds, vol. 619, pp. 834–838, 2015. View at: Publisher Site  Google Scholar
 S. Mandal, V. Rakesh, P. V. Sivaprasad, S. Venugopal, and K. V. Kasiviswanathan, “Constitutive equations to predict high temperature flow stress in a Timodified austenitic stainless steel,” Materials Science and Engineering A, vol. 500, no. 12, pp. 114–121, 2009. View at: Publisher Site  Google Scholar
 M. He, F. Li, and N. Ali, “A normalized damage variable for ductile metals based on toughness performance,” Materials Science and Engineering A, vol. 528, no. 3, pp. 832–837, 2011. View at: Publisher Site  Google Scholar
 S. Mandal, P. V. Sivaprasad, S. Venugopal, and K. P. N. Murthy, “Artificial neural network modeling to evaluate and predict the deformation behavior of stainless steel type AISI 304L during hot torsion,” Applied Soft Computing Journal, vol. 9, no. 1, pp. 237–244, 2009. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2015 Jinghui Li et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.